# Instrument Report: X-ray Diffraction Guanghui Zhu.

## Presentation on theme: "Instrument Report: X-ray Diffraction Guanghui Zhu."— Presentation transcript:

Instrument Report: X-ray Diffraction Guanghui Zhu

Contents Diffraction Mechanism Construction of the Diffractometer
Applications of XRD Data Analysis and Explanation 2D XRD XRD Simulation

Diffraction Mechanism

Crystalline materials are characterized by the orderly periodic arrangements of atoms.
The (200) planes of atoms in NaCl The (220) planes of atoms in NaCl The unit cell is the basic repeating unit that defines a crystal. Parallel planes of atoms intersecting the unit cell are used to define directions and distances in the crystal. These crystallographic planes are identified by Miller indices. Crystalline materials are characterized by the orderly periodic arrangements of atoms. Image: rpp.nashaucheba.ru/docs/index html

The atoms in a crystal are a periodic array of coherent scatterers and thus can diffract light.
Diffraction occurs when each object in a periodic array scatters radiation coherently, producing concerted constructive interference at specific angles. The electrons in an atom coherently scatter light. The electrons interact with the oscillating electric field of the light wave. Atoms in a crystal form a periodic array of coherent scatterers. The wavelength of X rays are similar to the distance between atoms. Diffraction from different planes of atoms produces a diffraction pattern, which contains information about the atomic arrangement within the crystal X Rays are also reflected, scattered incoherently, absorbed, refracted, and transmitted when they interact with matter.

Bragg’s law λ=2dhklsinθ q dhkl
For parallel planes of atoms, with a space dhkl between the planes, constructive interference only occurs when Bragg’s law is satisfied. In our diffractometers, the X-ray wavelength l is fixed. Consequently, a family of planes produces a diffraction peak only at a specific angle q. Additionally, the plane normal must be parallel to the diffraction vector Plane normal: the direction perpendicular to a plane of atoms Diffraction vector: the vector that bisects the angle between the incident and diffracted beam The space between diffracting planes of atoms determines peak positions. The peak intensity is determined by what atoms are in the diffracting plane.

dhkl

Miller index Miller indices form a notation system in crystallography for planes in crystal (Bravais) lattices. Image: DeepKling

A single crystal specimen would produce only one family of peaks in the diffraction pattern.
2q The (200) planes are parallel to the (100) planes. Therefore, they also diffract for this crystal. Since d200 is ½ d100, they appear at 42 °2q. At 20.6 °2q, Bragg’s law fulfilled for the (100) planes, producing a diffraction peak. The (110) planes would diffract at 29.3 °2q; however, they are not properly aligned to produce a diffraction peak (the perpendicular to those planes does not bisect the incident and diffracted beams). Only background is observed.

A polycrystalline sample should contain thousands of crystallites.
2q 2q 2q For every set of planes, there will be a small percentage of crystallites that are properly oriented to diffract Basic assumptions of powder diffraction are that for every set of planes there is an equal number of crystallites that will diffract and that there is a statistically relevant number of crystallites, not just one or two.

Construction of the Diffractometer

Essential Parts X-ray Tube: the source of X Rays
Incident-beam optics: condition the X-ray beam before it hits the sample The goniometer: the platform that holds and moves the sample, optics, detector, and/or tube The sample & sample holder Receiving-side optics: condition the X-ray beam after it has encountered the sample Detector: count the number of X Rays scattered by the sample

Bragg-Brentano geometry
The incident angle, w, is defined between the X-ray source and the sample. The diffracted angle, 2q, is defined between the incident beam and the detector angle. The incident angle w is always ½ of the detector angle 2q . In a q:2q instrument (e.g. Rigaku RU300), the tube is fixed, the sample rotates at q °/min and the detector rotates at 2q °/min. In a q:q instrument (e.g. PANalytical X’Pert Pro), the sample is fixed and the tube rotates at a rate -q °/min and the detector rotates at a rate of q °/min. Image:

X-radiation Sealed X-ray tubes tend to operate at 1.8 to 3 kW.
Rotating anode X-ray tubes produce much more flux because they operate at 9 to 18 kW. A rotating anode spins the anode at 6000 rpm, helping to distribute heat over a larger area and therefore allowing the tube to be run at higher power without melting the target. Both sources generate X rays by striking the anode target wth an electron beam from a tungsten filament. The target must be water cooled. The target and filament must be contained in a vacuum.

The wavelength of X rays is determined by the anode of the X-ray source.
Electrons from the filament strike the target anode, producing characteristic radiation via the photoelectric effect. The anode material determines the wavelengths of characteristic radiation. While we would prefer a monochromatic source, the X-ray beam actually consists of several characteristic wavelengths of X rays. K L M

Spectral Contamination in Diffraction Patterns
Ka1 Ka2 Kb W La1 Ka1 Ka2 The Ka1 & Ka2 doublet will almost always be present Very expensive optics can remove the Ka2 line Ka1 & Ka2 overlap heavily at low angles and are more separated at high angles W lines form as the tube ages: the W filament contaminates the target anode and becomes a new X-ray source W and Kb lines can be removed with optics

Copper Anodes Bearden (1967) Holzer et al. (1997) Cobalt Cu Ka1 Å Å Co Ka1 Å Å Cu Ka2 Å Å Co Ka2 Å Å Cu Kb Å Å Co Kb Å Å Molybdenum Chromium Mo Ka1 Å Å Cr Ka1 Å Å Mo Ka2 Å Å Cr Ka2 Å Å Mo Kb Å Å Cr Kb Å Å Often quoted values from Cullity (1956) and Bearden, Rev. Mod. Phys. 39 (1967) are incorrect. Values from Bearden (1967) are reprinted in international Tables for X-Ray Crystallography and most XRD textbooks. Most recent values are from Hölzer et al. Phys. Rev. A 56 (1997)

The X-ray Shutter--important safety device on a diffractometer
X-rays exit the tube through X-ray transparent Be windows. X-Ray safety shutters contain the beam so that you may work in the diffractometer without being exposed to the X-rays. Being aware of the status of the shutters is the most important factor in working safely with X rays.

The X-ray divergence λ=2dhklsinθ X Rays from an X-ray tube are:
divergent contain multiple characteristic wavelengths as well as Bremsstrahlung radiation neither of these conditions suit our ability to use X rays for analysis the divergence means that instead of a single incident angle q, the sample is actually illuminated by photons with a range of incident angles. the spectral contamination means that the smaple does not diffract a single wavelength of radiation, but rather several wavelengths of radiation. Consequently, a single set of crystallographic planes will produce several diffraction peaks instead of one diffraction peak. Optics are used to: limit divergence of the X-ray beam refocus X rays into parallel paths remove unwanted wavelengths

The X-ray divergence slit
Divergence slits are used to limit the divergence of the incident X-ray beam. The slits block X-rays that have too great a divergence. The size of the divergence slit influences peak intensity and peak shapes. Narrow divergence slits: reduce the intensity of the X-ray beam reduce the length of the X-ray beam hitting the sample produce sharper peaks the instrumental resolution is improved so that closely spaced peaks can be resolved.

Monochromators Diffraction from a crystal monochromator can be used to select one wavelength of radiation and provide energy discrimination. An incident-beam monochromator might be used to select only Ka1 radiation for the tube source. A diffracted-beam monochromator may be used to remove fluoresced photons, Kb, or W-contimination photons from reaching the detector. Without the RSM slit, the monochromator removes ~75% of unwanted wavelengths of radiation. When the RSM slit is used, over 99% of the unwanted wavelengths of radiation can be removed from the beam.

Detectors Point detectors Position sensitive detectors (PSD)
observe one point of space at a time slow, but compatible with most/all optics scintillation and gas proportional detectors count all photons, within an energy window, that hit them Si(Li) detectors can electronically analyze or filter wavelengths Position sensitive detectors (PSD) linear PSDs observe all photons scattered along a line from 2 to 10° long 2D area detectors observe all photons scattered along a conic section gas proportional (gas on wire; microgap anodes) limited resolution, issues with deadtime and saturation CCD limited in size, expensive solid state real-time multiple semiconductor strips high speed with high resolution, robust

Applications of XRD

Typical 1D Diffraction

You can use XRD to determine
Phase Identification Quantitative Phase Analysis: determine the relative amounts of phases in a mixture by referencing the relative peak intensities Unit cell lattice parameters and Bravais lattice symmetry Index peak positions Lattice parameters can vary as a function of, and therefore give you information about, alloying, doping, solid solutions, strains, etc. Residual Stress (macrostrain) Crystal Structure By Rietveld refinement of the entire diffraction pattern Epitaxy/Texture/Orientation Crystallite Size and Microstrain Indicated by peak broadening Other defects (stacking faults, etc.) can be measured by analysis of peak shapes and peak width In-situ XRD

Phase Identification The diffraction pattern for every phase is as unique as your fingerprint Phases with the same chemical composition can have drastically different diffraction patterns. Use the position and relative intensity of a series of peaks to match experimental data to the reference patterns in the database

Phase Identification The PDF (Powder Diffraction File) contains over 200,000 diffraction patterns. Modern computer programs can help you determine what phases are present in your sample by quickly comparing your diffraction data to all of the patterns in the database. The PDF card for an entry contains a lot of useful information, including literature references.

Quantitative Phase Analysis
With high quality data, you can determine how much of each phase is present must meet the constant volume assumption (see later slides) The ratio of peak intensities varies linearly as a function of weight fractions for any two phases in a mixture need to know the constant of proportionality RIR method is fast and gives semi-quantitative results Whole pattern fitting/Rietveld refinement is a more accurate but more complicated analysis

Unit Cell Lattice Parameter Refinement
By accurately measuring peak positions over a long range of 2theta, you can determine the unit cell lattice parameters of the phases in your sample alloying, substitution doping, temperature and pressure, etc. can create changes in lattice parameters that you may want to quantify use many peaks over a long range of 2theta so that you can identify and correct for systematic errors such as specimen displacement and zero shift measure peak positions with a peak search algorithm or profile fitting profile fitting is more accurate but more time consuming then numerically refine the lattice parameters

Residual Stress

Epitaxy/Texture/Orientation
Preferred orientation of crystallites can create a systematic variation in diffraction peak intensities can qualitatively analyze using a 1D diffraction pattern a pole figure maps the intensity of a single peak as a function of tilt and rotation of the sample this can be used to quantify the texture (111) (311) (200) (220) (222) (400) 40 50 60 70 80 90 100 Two-Theta (deg) x10 3 2.0 4.0 6.0 8.0 10.0 Intensity(Counts) > Gold - Au

Crystallite Size and Microstrain
Crystallites smaller than ~120nm create broadening of diffraction peaks this peak broadening can be used to quantify the average crystallite size of nanoparticles using the Scherrer equation must know the contribution of peak width from the instrument by using a calibration curve Microstrain may also create peak broadening analyzing the peak widths over a long range of 2theta using a Williamson-Hull plot can let you separate microstrain and crystallite size 23 24 25 26 27 28 29 30 31 32 33 34 35 36 37 38 39 40 41 2 q (deg.) Intensity (a.u.) > Cerianite- - CeO

Data

Diffraction patterns are best reported using dhkl and relative intensity rather than 2q and absolute intensity. The peak position as 2q depends on instrumental characteristics such as wavelength. The peak position as dhkl is an intrinsic, instrument-independent, material property. Bragg’s Law is used to convert observed 2q positions to dhkl. The absolute intensity, i.e. the number of X rays observed in a given peak, can vary due to instrumental and experimental parameters. The relative intensities of the diffraction peaks should be instrument independent. To calculate relative intensity, divide the absolute intensity of every peak by the absolute intensity of the most intense peak, and then convert to a percentage. The most intense peak of a phase is therefore always called the “100% peak”. Peak areas are much more reliable than peak heights as a measure of intensity.

Powder diffraction data consists of a record of photon intensity versus detector angle 2q.
Diffraction data can be reduced to a list of peak positions and intensities Each dhkl corresponds to a family of atomic planes {hkl} individual planes cannot be resolved- this is a limitation of powder diffraction versus single crystal diffraction Raw Data Reduced dI list Position [°2q] Intensity [cts] hkl dhkl (Å) Relative Intensity (%) {012} 3.4935 49.8 {104} 2.5583 85.8 {110} 2.3852 36.1 {006} 2.1701 1.9 {113} 2.0903 100.0 {202} 1.9680 1.4

Sample Preparation

Preparing a powder specimen
An ideal powder sample should have many crystallites in random orientations the distribution of orientations should be smooth and equally distributed amongst all orientations If the crystallites in a sample are very large, there will not be a smooth distribution of crystal orientations. You will not get a powder average diffraction pattern. crystallites should be <10mm in size to get good powder statistics Large crystallite sizes and non-random crystallite orientations both lead to peak intensity variation the measured diffraction pattern will not agree with that expected from an ideal powder the measured diffraction pattern will not agree with reference patterns in the Powder Diffraction File (PDF) database

Preferred orientation
If the crystallites in a powder sample have plate or needle like shapes it can be very difficult to get them to adopt random orientations top-loading, where you press the powder into a holder, can cause problems with preferred orientation In samples such as metal sheets or wires there is almost always preferred orientation due to the manufacturing process For samples with systematic orientation, XRD can be used to quantify the texture in the specimen

Important characteristics of samples for XRPD
a flat plate sample for XRPD should have a smooth flat surface if the surface is not smooth and flat, X-ray absorption may reduce the intensity of low angle peaks parallel-beam optics can be used to analyze samples with odd shapes or rought surfaces Densely packed Randomly oriented grains/crystallites Grain size less than 10 microns ‘Infinitely’ thick

Way to prepare a powder sample
Top-loading a bulk powder into a well deposit powder in a shallow well of a sample holder. Use a slightly rough flat surface to press down on the powder, packing it into the well. using a slightly rough surface to pack the powder can help minimize preferred orientation mixing the sample with a filler such as flour or glass powder may also help minimize preferred orientation powder may need to be mixed with a binder to prevent it from falling out of the sample holder alternatively, the well of the sample holder can be coated with a thin layer of vaseline

2D XRD

Introduction Two-dimensional x-ray diffraction (XRD2) refers to x-ray diffraction applications with two dimensional (2D) detector and corresponding data reduction and analysis. In addition to the 2D detector technology, it involves 2D image processing and 2D diffraction pattern manipulation and interpretation. The diffracted rays from a single crystal point to discrete directions each corresponding to a family of diffraction planes (Figure 2a). The diffraction pattern from a polycrystalline (powder) sample forms a series diffraction cones if large number of crystals oriented randomly in the space are covered by the incident x-ray beam (Figure 2b). Each diffraction cone corresponds to the diffraction from the same family of crystalline planes in all the participating grains Image: Bruker Analytical X-ray Systems

Components An XRD2 system is a diffraction system with the capability of acquiring diffraction pattern in 2D space simultaneously and analyzing 2D diffraction data accordingly. A two-dimensional x-ray diffraction system consists of at least one two-dimensional detector, x-ray source, x-ray optics, sample positioning stage, sample alignment and monitoring device as well as corresponding computer control and data reduction and analysis software. Figure 1 is an example of an XRD2 system with five major components. Two-dimensional detector, x-ray source, x-ray optics, sample positioning stage, sample alignment and monitoring device as well as corresponding computer control and data reduction and analysis software Image: Bruker Analytical X-ray Systems

XRD vs. XRD2 Image: Bruker Analytical X-ray Systems

2D Diffraction image Polycrystalline thin film on a single crystal substrate Mixture of fine and coarse grains in a metallic alloy Conventional linear diffraction patterns would miss information about single crystal or coarse grained materials

Sample Rotation Image: Bruker Analytical X-ray Systems

Applications Phase identification (Phase ID) can be done by integration over a selected range of 2θ and γ. The integrated data gives better intensity and statistics for phase ID and quantitative analysis, especially for those samples with texture, large grain size, or small quantity. Texture measurement is extremely fast. An XRD2 system collects texture data and background values simultaneously for multiple poles and multiple directions. Due to the high measurement speed, Pole figure can be measured at very fine steps for sharp textures. Stress can be measured using the 2D fundamental equation, which gives the direct relationship between the stress tensor and the diffraction cone distortion. Since the whole or a part of the Debye ring is used for stress calculation, it can measure stress with high sensitivity, high speed and high accuracy. It is very suitable for large grain and textured samples. Percent crystallinity can be measured faster and more accurately with the data analysis over the 2D pattern, especially for samples with anisotropic distribution of crystalline orientation.

Applications(cont’d)
Small angle x-ray scattering (SAXS) data can be collected at high speed. Anisotropic features from specimens, such as polymers, fibrous materials, single crystals and bio-materials, can be analyzed and displayed in two-dimension. De-smearing correction is not necessary due to the collimated point x-ray beam. Since one exposure takes all the SAXS information, it is easy to scan over the sample to map the structure information. Microdiffraction data is collected with speed and accuracy. The 2D detector captures whole or a large portion of the diffraction rings, so spotty, textured, or weak diffraction data can be integrated over the selected diffraction rings. Thin film samples with a mixture of single crystal, random polycrystalline layers and highly textured layers can be measured with all the features appearing simultaneously in 2D frames.

XRD Simulation

Bragg’s Law

dhkl

Scattering Amplitude--Structure Factor F

Scattering Amplitude-- Scattering Factor f

Peak Width Peak Width B(2q) varies inversely with crystallite size
𝐵 2𝜃 = 𝐾𝜆 𝐿𝑐𝑜𝑠𝜃 Peak Width B(2q) varies inversely with crystallite size The constant of proportionality, K (the Scherrer constant) depends on the how the width is determined, the shape of the crystal, and the size distribution The most common values for K are 0.94 (for FWHM of spherical crystals with cubic symmetry), 0.89 (for integral breadth of spherical crystals with cubic symmetry, and 1 (because 0.94 and 0.89 both round up to 1). K actually varies from 0.62 to 2.08 For an excellent discussion of K, JI Langford and AJC Wilson, “Scherrer after sixty years: A survey and some new results in the determination of crystallite size,” J. Appl. Cryst. 11 (1978) p

Diffraction Pattern

Where to Get Crystal Structures

Software for Simulation
PANalytical X’Pert HighScore Plus With the crystal structure information, we can build a crystal in HSP Then we can simulate the ideal X-Ray powder diffraction pattern in HSP The pattern simulation parameters can be changed in Program Settings We can change parameters for the crystal structure and observe how they change the diffraction pattern

Note These simulations do not necessarily represent the data that your diffractometer will produce There are more factors that contribute to the diffraction pattern that you collect with an instrument Some of these factors are calculated from fundamental equations The simulations that we have been executing already account for multiplicity, for Ka2 radiation, and for the Lorentz polarization factor Some of these factors are approximated using empirical formulas The simulations that we have been executing already account for the peak width due to divergence, mosaicity, resolution of the diffractometer

Supplementation

XRD @ UMD http://www2.chem.umd.edu/facility/xray
Chemical Crystallography lab Bruker Apex2 Bruker Smart1000 Materials Characterization lab Bruker C2 Discover Bruker D8 Advance Protein Crystallography lab Bruker Proteum X8 (coming soon)

Recommend Readings Elements Of X Ray Diffraction, B.D.Cullity
Fundamentals of Powder Diffraction and Structural Characterization of Materials, Second Edition, Vitalij K. Pecharsky and Peter Y. Zavalij Collection of Simulated XRD Powder Patterns for Zeolites, M.M.J. Treacy and J.B. Higgins, IZA

Useful Software MDI Jade PANalytical HighScore Plus PANalytical Stress
PANalytical Texture PANalytical Reflectivity Bruker Multex Area

Thank You!

Download ppt "Instrument Report: X-ray Diffraction Guanghui Zhu."

Similar presentations